- Review article
- Open Access
Pulsed Eddy Current Non-destructive Testing and Evaluation: A Review
© Chinese Mechanical Engineering Society and Springer-Verlag Berlin Heidelberg 2017
- Received: 2 November 2016
- Accepted: 28 March 2017
- Published: 17 April 2017
The Erratum to this article has been published in Chinese Journal of Mechanical Engineering 2017 30:177
Pulsed eddy current (PEC) non-destructive testing and evaluation (NDT&E) has been around for some time and it is still attracting extensive attention from researchers around the globe, which can be witnessed through the reports reviewed in this paper. Thanks to its richness of spectral components, various applications of this technique have been proposed and reported in the literature covering both structural integrity inspection and material characterization in various industrial sectors. To support its development and for better understanding of the phenomena around the transient induced eddy currents, attempts for its modelling both analytically and numerically have been made by researchers around the world. This review is an attempt to capture the state-of-the-art development and applications of PEC, especially in the last 15 years and it is not intended to be exhaustive. Future challenges and opportunities for PEC NDT&E are also presented.
- Non-destructive testing
- Pulsed eddy currents
- Material characterization
- Structural integrity
- Non-destructive evaluation
Despite its approximately-five-decade-long history, PEC is still considered by many as a new emerging eddy current NDT&E technique. Compared to other eddy current testing (ECT) techniques this view can be true. Literature shows that PEC has been attracting the attention of researchers from around the globe, including countries, such as China, UK, Canada, Portugal, USA, South Korea, Japan, France, Slovakia, Poland, and Italy.
The amount of attention that PEC NDT&E has been receiving owes to the key potential benefits that it offers. The first and main advantage is that, compared to single frequency ECT, PEC inherently has a broadband of frequencies , which is advantageous for any eddy-current-based NDT&E techniques due to the frequency-dependant skin effect. Another benefit is that PEC signals are relatively easier to interpret, while it requires a special skill of the operators for interpreting conventional ECT signals which are presented in the impedance plane trajectory.
Similar to other ECT techniques, in general PEC requires no surface preparation which leads to reduction of inspection time and costs efficiency is improved. The inspection can also be done without interrupting the operation or service of the structure being tested, unlike for example X-ray testing. In many applications where the sample is coated, no removal of the coating is required when ECT NDT&E is used. Any eddy-current systems are relatively cost-effective and reliable.
In the following sections, the concept of PEC is briefly discussed which is then followed by the review in systems, modelling, signal processing and applications. A conclusion completes this review paper.
From one implementation to another, the systems vary primarily because of the differences in the excitation signal, excitation system, sensing device and the signal processing and feature extraction techniques. These variations are discussed below.
3.1 Excitation Signals
Typically, a PEC probe would contain one excitation coil and one or more sensing devices. An excitation coil generates primary transient excitation field, while one or more sensing devices picks up secondary eddy current field due to a sample. Probe designs are usually optimized in terms of its structure, the type of sensing elements and the use of cores based on the specific applications in which they will be deployed.
Differential probes, as opposed to absolute probes, are also used with the advantage of the self-nulling features and therefore no reference signals are required. This type of probe can be implemented by using two pick-up coils or two magnetic sensors with the output signal being the difference between the two output signals from the sensing devices. A differential double-D probe using two Hall devices has been investigated by Park, et al  which shows a potential for detection and sizing of sub-surface cracks in stainless-steel structures. Differential probes have also been studied for crack detection near a fastener in aircraft structures , .
Another differentiating feature is the shape of the coil. Rather than being circular, which is the most common shape, the coil may be rectangular or racetrack. This non-circular type of a coil is also referred as directional as opposed to non-directional or isotropic for circular coils. With directional probes, the paths of the induced eddy currents are not circular, and, therefore, they are more sensitive to changes in a particular direction. One example of the use of directional rectangular coil is the work done by He, et al , . They also state that a more uniform eddy current distribution is being an advantage gained by using such a coil.
A ferromagnetic core and shielding maybe present with the purpose of concentrating the magnetic flux and amplifying the signal. Hence, for enhancement of the sensitivity of the probe in certain applications, a ferromagnetic core or shielding is added to the probe. An example of the study in this topic is introduced in Ref. , where the sensitivity in sub-surface detection was evaluated. The study, which uses both numerical modelling and experimental tests, shows a favour for a ferrite-cored but unshielded over a shielded, ferrite-cored probe. A study by Zhou, et al  shows that a shield made of iron, that is positioned between the excitation coil and the magnetic sensor, provides a higher sensitivity compared with non-shielded and aluminium-shielded probes for ferromagnetic inspection.
3.3 Sensing Devices
The output signal of an induction coil depends on the rate of change of magnetic flux density, while that of a magnetic sensor is directly proportional to magnetic flux density. As a result, the response from an induction coil exhibits similar characteristics with that of a magnetic sensor . Each of these types has its own advantages and disadvantages. Induction coils play a dominant role in use for simplicity of operation and design, wide frequency bandwidth and large dynamics. However, induction coils are only sensitive to AC magnetic field, which is one of the drawbacks, although this drawback could be handled by introducing movement to the coil . Magnetic sensors are typically sensitive to low frequency signals and offer a better spatial resolution. Hence, magnetic sensors have gained wide acceptance for enhancement of sensitivity and spatial resolution in sensing low frequency magnetic field . In the applications where extremely high temperatures are involved, induction coils can be the only feasible option.
There are various types of magnetic field sensors available nowadays. Accumulatively, they can sense field from as low as in the order of several 10−15 T up to around 100 mT . In PEC NDT, the most widely used magnetic sensors are Hall effect devices (e.g., Ref. ) and magnetoresistive (MR) devices. Both of these sensor types are relatively low cost. Hall effect devices have the highest dynamic range, covering approximately 100 μT up to 100 mT, however they have high noise, low resolution and low sensitivity.
Out of three existing types of MR technologies, two types are used in PEC NDT, which are anisotropic magnetoresistance or AMR(e.g., Ref. ) and giant magnetoresistance or GMR (e.g., Ref. ). The use of the latest development of MR, i.e., tunnelling magnetoresistance (TMR), in PEC systems has not been found by the authors in any literature despite it has the highest sensitivity. The lack of the presence if TMR in PEC systems may be due to its relatively new availability. While its technology is still being improved, an analysis – that may be rather outdated now - shows that despite its higher sensitivity compared with AMR and GMR, its detectivity is not necessarily higher due to its higher 1/f noise . The detectivity signifies the lowest magnetic field a sensor can detect, where the signal-to-noise ratio is unity. However, it is expected that further development of TMR will improve its detectivity and may make it more interesting for PEC applications.
Another type of magnetic field sensor, namely high temperature superconducting quantum interference device (HTS SQUID) magnetometer has also been studied in PEC . SQUID has the highest sensitivity with the ability of measuring in the range down to 10−15 T, however its applications in NDT is still limited due to its practicality and costs.
Whilst most of sensing devices used are absolute, the use of gradient-field GMR sensors has also been reported by Li, et al . Interestingly, they discover that the gradient-field measurements give better sensitivity and accuracy in detection and sizing artificial sub-surface corrosion in layered samples. Typically, two measurement points are deployed in gradient-field sensing. The two points stand at two different z-distances to the specimen under test.
Additionally, Joubert, et al have studied the use of magneto-optical (MO) film for imaging the structure of riveted multi-layered aircraft assembly for detecting cracks that are emanating from the rivet in hidden layers of the structure , . The film is affected by the distribution of the magnetic fluxes induced by the eddy current and will reflect the light deliberately shone on it towards a CCD camera.
In terms of the direction of the field that is measured, most probes would detect field normal to the surface of the sample under test. However, there are also probes that are designed to detect the field parallel to the surface, such as the work in .
PEC’s electromagnetic problems, just like other eddy current NDT&E methods, are governed by Maxwell equations. They can be solved in both time and frequency domains. For frequency domain solutions, the time-based signals are transformed first into frequency spectrum by using Fourier transform before later, having gone through some processing, transformed back into the time domain in order to get the final results. As with many other engineering problems, both analytical and numerical models are used in PEC. Analytical methods are known to be fast in the processing, although they are used only for relatively simple geometries. Reports show that researchers have attempted to build and use both analytical and numerical models for PEC since 1980’s [36–39], with the initial objective of gaining better understanding of the PEC phenomena when used in NDT inspection. Therefore, the relative success in the modelling of PEC has allowed the advancement of PEC and its successful application to many different problems. In the following paragraphs, a few examples of works dealing with PEC modelling are mentioned with no intention for delving into details.
Recently, Desjardins, et al have presented an analytical approach ,  to model an encircling coil used around a ferromagnetic rod. The method computes the time-domain electromagnetic response of the system and the results were validated by experimental data that display a very good agreement. Increasingly, a method for determining the electrical conductivity and the magnetic permeability that arises from the analytical solution for the ferromagnetic rod and encircling coils has been also suggested by Desjardins et al . This is a good example of how modelling may enhance the use of PEC in NDT inspection.
For the measurement of the wall thickness of pipes, another analytical method relying on the use of inverse Laplace transform has been developed in Ref. . The model is, unlike most reported analytical models, non-axisymmetric and it presents a good correlation with measured data. Rather than having an encircling coil, the excitation coil is perpendicular to the surface of the pipe. For complex cases, numerical algorithms like Stehfest and Fast Fourier transform have been proposed to do the inversion of Laplace transform, because analytical inversion of Laplace transform is inaccessible . Chen et al also proposed new signal features that can be used for determining the sample plate’s magnetic permeability and electrical conductivity assuming that the thickness is previously determined by means of their analytical model .
An analytical model based on the Fourier superposition concept has been presented for modelling the crack detection task in a multi-layered structure and validated by using FEM results . Accuracy of the model in the results has been shown with fast execution time compared to the FEM solution. An example of the use of numerical model is introduced in Ref. , which studies PEC signals when corrosion occurs in the inner wall of an insulated pipe. The signal features such as peak and zero crossing times were investigated by using the FEM model. Another example of reported work on numerical was presented in Ref.  that used the Fourier transform rather than time-stepping. The validation of the model was carried out by using experimental data at selected frequencies for detection of denting problems.
PEC signals, as conventional ECT, are affected by various factors, such as electrical conductivity, lift-off, magnetic permeability, thickness of the sample and inhomogeneity of the material. The other challenges faced by researchers in obtaining useful information from the signals are the noise and the low level signals in some cases. Consequently, the right signal processing, signal analysis, feature extraction and classification model must be implemented in order to attain the desired parameters, such as coating thickness, size and position of defects, and to isolate them from the undesired parameters, such as lift-off variation.
5.1 Signal Feature and Feature Extraction
The features that are used to infer the desired parameters may be readily available, such as peak value , , , peak arrival time , rising time  and zero crossing time . In addition to these more traditional features, there have also been emerging features proposed in various reports, such as the so called “relative variation of magnetic flux” , which has been shown through both simulation and experiments to have potentials in determining the lift-off for ferromagnetic materials . This feature is calculated by processing an interval of the decay part of the field is used rather than the rising part and it should not, nevertheless, be used for small lift-offs. Huang et al discussed another feature derived from the cumulative integration of the time signal from the decaying part . The feature is related to the time constant of the first order component of the signal and it is used to predict the thickness of ferromagnetic plates. Another example is the kurtosis coefficient, which represents the craggedness level of a PEC response signal, that is used in sample’s edge identification .
In other cases, researchers try to optimise the discrimination within the range of the parameters, which require them to employ data dimensionality reduction techniques. In some of the cases, the obtained features are subsequently fed into a classifier in order to either classify or quantify the defects.
Dimensionality reduction techniques used in the feature extraction for PEC signals that have been reported include principal component analysis (PCA), independent component analysis (ICA)  and Fisher linear discriminant analysis (FLDA) . PCA has been the most widely used since the work of Tian, et al that was reported in . Other examples of work where PCA has been used are introduced in Refs. , , , , [55–60].
The input data that are fed into the feature extraction stage can be time domain signals, frequency domain signals or the combination of both domains. Examples of time domain signal input are captured in Refs. , , .
In addition to the time domain features, frequency domain features are also utilized, both with and without the use of the time domain ones. This is understandable as PEC signals contain a wide spectrum of frequencies. And considering the skin depth effect, it is widely known that higher frequencies are more sensitive to surfer or near surface defects, while lower frequencies penetrated deeper resulting in sensitivity to more deeply buried defects.
For classification of surface and sub-surface defects, He, et al  used amplitudes of a few harmonics generated by using FFT. In another more recent work, for mapping artificial surface slots and holes, Abrantes, et al have also used FFT to get the amplitudes and phases of the fundamental and harmonics . By using the amplitudes and phases of selected frequencies, the defects can be identified. The phases are shown to pinpoint the centre of the defect when they swing by 180°. The very high frequencies that are used should mean that only surface defects can be dealt with the approach.
Another example of FFT-based work is done in Ref. , which shows the ability to discriminate different types of defects, namely surface crack, sub-surface crack, surface cavity and sub-surface cavity. An improved result is, however, shown when the time signal is decomposed first by using wavelet into the approximate and detail signals before being transformed into the frequency domain by using the FFT. PCA is then used in order to extract the most significant features to be used for the classification stage.
Power spectral density analysis (PSDA) is also used by Qiu, et al  as frequency-domain features, which are believed by the authors to be more stable and accurate in the extraction than time domain features, citing the work  that uses spectral amplitude and phase as the signal features.
Finally, there are many works where both time and frequency domain features are used simultaneously. Within this group, time–frequency decomposition tools are often used, such as Wavelet, empirical mode decomposition (EMD) and Rihaczek distribution. Following the analysis, a feature extraction technique, such as PCA and Fisher linear discriminant analysis (FLDA), is then normally used in order to reduce the data dimensions for defect classification purposes.
Tian, et al used wavelet transform, which captures both temporal and spectral information from the time signals of PEC, in order to improve their classification . Hosseini and Lakis use Rihaczek distribution for time–frequency analysis of the signals and follow it up using PCA to reduce the features, which are the used classify defects located in different layers in a multi-layered specimen .
The use of both time and frequency domains is studied by Ref.  for detection and characterization of cracks under fasteners in aircraft layered-structures. The combination of the signal analysis and unique symmetric excitation coil leads to the ability in detection of 1 mm-long crack at the depth of 10 mm aided by a GMR sensor. Although in the study, the time and frequency domain features were presented separately, the combination of both may increase the confidence in the detection.
Zhang, et al combines both time domain features, namely peak value, peak time and rising time, together with a frequency domain feature derived by using EMD and Hilbert transform for classification of surface notch, sub-surface notches and wall losses . In this work, the researchers do not need to use any data dimensionality reduction.
As mentioned earlier, in many cases researchers have proposed the use of a classifier for classification or quantification of defects. It is thought that this would be an important and desirable feature for future PEC systems that will potentially reduce the level of operator skill requirements. An automated system that will reliably provide information on the location and type or size of a detected defect would be advantageous which reduce dependency on human interpretation skills.
Broadly, there are two major groups of classification methods, which are supervised and unsupervised. In supervised classification, the training data are labelled based on the class, such as defect type or location. On the other hand, unsupervised classification does not require the labelling of the training data, therefore this classification is really only clustering the input data without identifying what each cluster represents.
Both categories of classification have been studied and used in PEC NDT. The supervised classification methods include support vector machine (SVM) and Linear Discriminant Analysis (LDA), whilst the used unsupervised include K-means and Bayes. In the majority of the reported works, neither classifying nor clustering methods have been used. Rather, manual human interpretation is made on the plots of distribution of the features.
There are only a few reports on the use of supervised classification, one of them is Ref. , where SVM techniques have been employed in conjunction with Fischer’s LDA (FLDA) for localization and classification of defects in multi-layered structure.
For unsupervised methods, K-means has been used for estimation of the size the cracks, also in aircraft structures . Another report by Qiu, et al  included both supervised and unsupervised methods, namely LDA and Bayes. Although they report both approaches managed to separate the surface and sub-surface defects, from the resulting plots it can be seen that the separation achieved by using LDA is better and has relatively wider distances between the two groups of defects.
5.3 Lift-off Problem
Lift-off problem has always been associated with eddy current NDT, and PEC is not an exception. The detrimental effect of lift-off slows down and limits the spread of the applications of PEC and ECT in NDT. Thankfully, many researchers have attempted to overcome this problem and proposed techniques to eliminate or reduce the effect of lift-off variation. Each of these techniques may only be applicable to specific PEC system implementations and applications.
The most popular features to be used in order to minimize the effects of lift-off is called lift-off point of intersection (LOI), which is a point at which PEC signals intersect when only lift-off distance varies. Therefore, LOI is inherently immune to lift-off variations, which makes a LOI point one of desirable features to remove lift-off effect for PEC evaluation. LOI phenomenon was originally observed in experiments and proposed to avoid false indication due to lift-off effect when material loss in a two-layer assembly was evaluated by PEC technique , . It is reported that the signals of LOI points have been successfully adopted to measure the thickness of a plate  and quantify defects and their locations in a layered sample . To enable the interpretation of LOI signals, the characteristics of LOI signals in terms of time and amplitude were revealed under a wide variety of conditions. The results demonstrate that LOI signals including both the time and amplitude follow a unique curve against thickness and conductivity . At the early stage, LOI phenomenon could only exist when a PEC probe using a coil as the receiver is placed above a nonferrous sample. Tian, et al  obtained LOI points by doing the derivative of the output of a Hall-based probe, and Li  extended the method to a PEC probe in which a solid-state magnetic field sensor could be placed at arbitrary positions. Further, Lefebvre and Mandache  recorded LOI phenomenon by covering a conductive but nonferrous layer on a ferromagnetic substrate. Also, Mandache and Lefebvre  made an attempt to disclose the physics of the LOI phenomenon. It is found that the LOI phenomenon is a general characteristic of the eddy currents, not only to transient eddy currents. Kral, et al  presented a linear transformer model to investigate the origin of LOI phenomenon, and obtained LOI points from the time derivatives of the output of a GMR-based probe. Interestingly, a LOI point is recently observed in the spectral PEC signals .
The use of normalisation and of two reference signals has been proposed to reduce the effects of lift-off . Tian, et al found that lift-off invariance (LOI) existed for magnetic sensors - not only for pick-up coils - and proposed new lift-off estimation techniques by using theoretical models . They believe that the techniques may also be used when an array of pick-up sensors are used.
A technique to indirectly reduce the effects of lift-off by using the slope of the difference signal has been proposed . The technique is potentially useful in the measurement of depth of surface defect.
The work done by Huang and Wu shows that the relative rate of change of the magnetic flux is independent of lift-off and, therefore, is a good candidate for getting the desired information from the PEC signals, which was in the inference of the thickness of ferromagnetic plates . The use of normalisation in frequency domain signals can also be used to reduce the effect of lift-off variation .
Thanks to its versatility, PEC NDT has been used in numerous different NDT applications, both in material characterization and structural integrity inspection. In material characterization, PEC has been suggested to be used for measurement of electrical conductivity and magnetic permeability of materials. Whilst, in the structural integrity testing, PEC NDT has been applied for defect detection and characterization, evaluation of corrosion, measurement of insulation thickness, plate thickness and wall thickness of pipe. This covers both insulated and non-insulated, coated and non-coated materials. Furthermore, still within the area of integrity testing, detection of cracks under fasteners and between fasteners in aircraft structures using PEC has also been explored and implemented. References to show the wide diversity of PEC applications are included and discussed briefly below.
6.1 Measurement of Electrical Conductivity and Magnetic Permeability
The use of PEC in the measurement of electrical conductivity of ferromagnetic materials, such as carbon steel plates, has been investigated by Chen, et al . They have successfully established PEC as a non-contacting measurement method with a maximum error of 1.6%. In a similar application, Desjardins, et al  mentioned in their study that the resulting conductivity from the transient eddy current is within 0.5 MS/m from that obtained by the four-point measurement. A carbon steel tube with wall thickness of 0.035’’ was used in their experiment, which was also supported by an analytical calculation with an excellent agreement. In the same work, they also showed a good result on the use of PEC in measurement of magnetic permeability.
6.2 Measurement of Thickness of Insulation and Coating
In ensuring its efficiency, the thickness of thermal insulation of vessels and pipes is an important parameter that needs to be monitored regularly in petrochemical industries. Experimental measurements of the thickness of thermal insulation on a steel plate has been done by using PEC and the report shows that an effective thickness measurement of up to 80 mm is possible .
In the area of coating thickness determination, Tai, et al obtained excellent results for both magnetic and non-magnetic coatings on both magnetic and non-magnetic substrates by using peak values . Their work was also supported by analytical theoretical models. Coating is very important for corrosion protection, among others.
6.3 Measurement of Thickness and Evaluation of Corrosion
Thickness measurement and evaluation of corrosion are discussed in the same section as basically the work on the same principle and the many of the works done in thickness measurement are intended for inspection of corrosion.
An example of the work in plate thickness measurement is introduced in Ref. , where a thickness of up to 30 mm was shown to be successfully measured. The plate was made of Q235 steel. Another example of work in this topic was presented by Shin, et al who investigated different materials, including copper, tungsten, inconel 600, aluminium and titanium .
Röntgen Technische Dienst(RTD) – now known as Applus RTD – has created a PEC system called RTD-Incotest that is able to measure the wall thickness – ranging from 6 mm up to 65 mm – of both pipes and plates made of low alloy carbon steel, even when they are under insulation of up to 150 mm in thickness . By measuring the wall thickness, the corrosion under insulation (CUI) can be evaluated.
Another company – Canada-based Eddyfi – has also made a commercial PEC system more recently. The system is capable of measuring wall thickness of up to 64 mm under non-magnetic and non-conductive insulation with thickness up to 203 mm . The testing can even be performed in the presence of conductive weather jackets of up to 1.5 mm thick (depending on the material). The ability of measuring wall thickness through the insulation and weather jacket is clearly a unique advantage for PEC systems.
Research works related to the estimation of pipe wall thickness include , , , and . A potentially effective method based on time-to-peak has been presented by Xu, et al for the assessment of wall thinning of insulated pipe . The time-to-peak feature divided by the thickness of a calibration sample is linearly related to wall thickness within 60% of the calibration sample . Such a feature is robust to thermal insulation and lift-off, which is verified by Park, et al . In a very similar type of application, Park et al studied the use of PEC to determine the wall thinning of stainless steel pipes in nuclear power plants without removing the insulation, where it could estimate thickness of up to 5 mm at the lift off of 6 mm . Huang, et al  and Cheng investigated the decay behaviour of logarithmic scaled PEC signals. It is found that the decay coefficient is approximately linear to wall thickness, and is insensitive to lift-off variations .
A distinctive approach by using a remote field probe has been presented in Ref.  for wall thickness measurement of ferromagnetic tubes from the inside. The researchers believe that this would be suitable for harsh-environment operation.
6.4 Detection and Characterization of Defects
There is a long list of literatures covering this topic, showing that it has been the main focus of researchers in PEC. For example, detection and sizing of sub-surface defects in a non-magnetic specimen made of AISI type 316 stainless steel has been shown in Ref. . The deepest notch was located 6 mm below the surface in an 8-mm-thick block. Works with similar types of artificial defects and similar shape of sample, i.e., plate or block, have also been reported by Tian, et al , , , .
Other examples of defect detection and characterization include flaws in the inner surface of pipe under insulation , outer corrosion on carbon steel pipes used in oil and gas industry , surface and sub-surface cracks and cavity detection in con-casting slabs (CCS) , subsurface corrosion in a plate , surface corrosion on coated mild steel S275 plates , , and various types of defect on steam generator support structures . Detection of wall thinning in pipe structures has been included in the previous sub-section above.
Aircraft industry has been given a lot of attention by the PEC research community since the very early stages of PEC history. Stress-induced cracks that occur under a fastener and between fasteners in multi-layered structures of the wings are crucial to be detected early for the safety of the aircraft during its flights. Works related to these issues can be found in the following works about PEC , , , , , , , , among others.
Related to the aircraft industry is the new emerging material carbon fiber reinforced plastic or CFRP for short. CFRP is growing in use in various industrial sectors thanks to its strength and lightness. However, its relative proneness to impact damage immediately leads to the industrial requirement of effective NDT techniques for ensuring its integrity. On the light of this, researchers have investigated the application of eddy current NDT, including PEC, to detect and characterize defects and damage in CFRP , . The CFRP problem is particularly challenging due to its anisotropic characteristic. It can be said that the achievement in this application is still limited.
An initial study of the possibility of measuring stress in aluminium alloy has been reported in Ref. , which concludes that further work should be done before the technique can be realized as an inspection tool. Another application in defect detection is one for friction stir welding .
The potential opportunities of PEC are shaped by both its strengths and the progressively more quantitative requirements of NDT&E, which is characterised by ever increasingly more stringent safety regulations; and this is especially true in the sectors where human lives are in stake, such as aerospace and nuclear industry. This would make the role of NDT&E even more important and relevant than ever. Opportunities for NDT in general and PEC in particular, are also presenting themselves as currently many structures and aircraft fleet are ageing, which need suitable and appropriate NDT inspections for ensuring safe and reliable operations with minimum downtimes.
A reliable, yet affordable technique will obviously be preferred by customers and operators alike. It is thought that the costs of the application of NDT can be reduced through enhanced sensitivity and improved user-friendliness, among others. With improved sensitivities, the interval between tests can be made longer and, therefore less tests need to be performed, which in turn, will help reduce the costs. This challenge presents an opportunity for PEC, especially in the optimisation and innovation related to the probe design, which should make the best use both analytical and numerical modelling methods. An example is the use a rather innovative a differential probe based on a rectangular excitation coil , that has been designed with the help of a finite element model. The probe successfully produces higher sensitivity in detection of defect in different materials, including CFRP.
The sensitivity of the PEC techniques may also be improved through the use of newer types of magnetic sensors, such as the tunnelling magnetoresistance (TMR), thanks to the continuous improvement in the sensitivity of magnetic sensing technologies. TMR exhibits a higher sensitivity and higher signal-to-noise ratio (SNR) compared with hall devices and other magnetoresisitive sensors, including GMR .
As for more user-friendly systems, they would be depending less on the high skills of the operators for interpreting the signals and the amount of training can be kept a minimum. All this, again, will help save the costs involved in in-service inspection for ensuring the integrity of structures or parts. Such systems can be materialized by having an automated classification for defects. The use of supervised classification techniques should be studied and developed more in order to give an answer to this challenge. Applications that may benefit from an automated classification functionality are those where multi types or locations of defects are potentially present, which include the inspection of aircraft multilayer structures and inspection of support structures in steam generators.
Cost reduction can also be achieved when the inspection time can be lowered. In this case, PEC may be able to benefit from the usage of multi-modal NDT and data fusion. This approach has not shown any significant appearance in the literature and new research can be undertaken to open up new opportunities for the application of PEC NDT. Another way of slashing the inspection time is, as already rising in popularity with some other NDT techniques, by the application of robotics. Again, opportunities in this area of research are still wide open for exploration, while there is only a handful of relevant existing literature.
In manufacturing industry, there is an increasing support for the use of NDT&E to improve the quality and consistency of the products. The potential ability of contactless thickness measurement of plates or sheets should be exploited so that PEC with its unique benefits can be used in manufacturing process control for such products. The ability of negating the effects of lift-off variations during measurement has to be achieved for generating consistently accurate results. If the required level of accuracy can be met, the PEC approach can be more advantageous compared with, for example, the use of laser triangulation sensors that would need access to both sides of the plates or sheets.
Simultaneous measurement of multiple parameters, such as conductivity, permeability and thickness is strongly demanding, and attracting increasingly more attention for quality control or structural integrity in some cases. In practice, multi-sensing modalities are performed for a comprehensive assessment, which is costly, labour-intensive and sometimes time-consuming. Fortunately, PEC is thought to be a feasible and efficient tool to measure conductivity, permeability and thickness simultaneously. Chen, et al  proposed an analytical-model-based method to infer conductivity and permeability with the prerequisite of knowing the wall thickness beforehand. Adewale, et al  investigated the contribution of permeability and conductivity on PEC signals. It is found that conductivity effects are prominent in the rising edge of the transient response, whereas permeability effects dominate in the steady stage. This finding presents a feasible way to decouple permeability and conductivity, and implies a feasible method to infer these two parameters within one measurement. Desjardins, et al  created a novel forward-solutions-based inverse method for simultaneous and accurate characterization of permeability and conductivity by computing the areas under scaled PEC signals. At present, the developed methods are only proven to be feasible. However, much work still needs to be done to make these methods applicable. For example, the developed methods need to be extended in order to be able to determine four or more parameters or be applied to a layered sample. Further, the accuracy of the existing methods greatly relies on the correlation between calculated and experimental data. The efforts to reduce the discrepancy should be made for accuracy improvement. In addition, uncertainty analysis should also be performed to evaluate the proposed methods .
PEC NDT&E has received a great deal of attention from researchers in the past 30 years and more, and yet, new applications and techniques are still being proposed and reported, as shown in this review. This gives approval to the theoretical understanding that PEC is rich of information that is potentially useful for quantitative NDT&E.
Literature on different aspects of PEC NDT has been presented and discussed. Challenges and opportunities of PEC NDT in the future have also been brought forward. It is expected that this work can contribute to research work in PEC NDT, especially for researchers and developers who are embarking a project in PEC NDT.
The authors would like to thank Ministry of Higher Education of Malaysia for funding the project on PEC NDT at IIUM through the research grant FRGS16-059-0558. This work is also supported by the National Natural Science Foundation of China under research grants 51677187 and 51307172. Dr. Mengbao Fan would like to thank China Jiangsu Provincial Department of Education and China University of Mining and Technology for sponsoring his visit to Newcastle University as an academic visitor.
- Lebrun B, Jayet Y, Baboux J-C. Pulsed eddy current signal analysis: application to the experimental detection and characterization of deep flaws in highly conductive materials. NDT E Int., 1997, 30(3): 163–170.Google Scholar
- Michniakova M, Janousek L. The impact of various waveform shapes on the response signal in pulsed eddy current NDE. ELEKTRO 2012, 2012: 439–442.Google Scholar
- Li J, Wu X, Zhang Q, et al. Pulsed eddy current testing of ferromagnetic specimen based on variable pulse width excitation. NDT E Int., 2015, 69: 28–34.Google Scholar
- Li Y, Yan B, Li D, et al. Pulse-modulation eddy current inspection of subsurface corrosion in conductive structures. NDT E Int., 2016, 79: 142–149.Google Scholar
- Abidin I Z, Mandache C, Tian G Y, et al. Pulsed eddy current testing with variable duty cycle on rivet joints. NDT E Int., 2009, 42(7): 599–605.Google Scholar
- Dolabdjian C P, Perez L, De Haan V O, et al. Performance of magnetic pulsed-eddy-current system using high dynamic and high linearity improved giant magnetoresistance magnetometer. IEEE Sensors Journal, 2006, 6(6): 1511–1517.Google Scholar
- Li J, Wu X, Zhang Q, et al. Measurement of lift-off using the relative variation of magnetic flux in pulsed eddy current testing. NDT E Int., 2015, 75: 57–64.Google Scholar
- Huang C, Wu X. An improved ferromagnetic material pulsed eddy current testing signal processing method based on numerical cumulative integration. NDT E Int., 2015, 69: 35–39.Google Scholar
- Blitz J. Eddy current testing of metails. NDT E Int., 1997, 30(1): 41.Google Scholar
- Desjardins D, Krause T W, Clapham L. Transient eddy current method for the characterization of magnetic permeability and conductivity. NDT E Int., 2016, 80: 65–70.Google Scholar
- Desjardins D R, Krause T W, Clapham L. Transient response of a driver coil in transient eddy current testing. NDT E Int., 2015, 73: 8–14.Google Scholar
- Vasic D, Bilas V, Ambrus D. Pulsed eddy-current nondestructive testing of ferromagnetic tubes. IEEE Transactions on Instrumentation and Measurement, 2004, 53(4): 1289–1294.Google Scholar
- Park D G, Angani C S, Cheong Y M. Differential pulsed eddy current probe to detect the sub surface cracks in a stainless steel pipe. 18th World Conference on Nondestructive Testing, 2012.Google Scholar
- Horan P, Underhill P R, Krause T W. Pulsed eddy current detection of cracks in F/A-18 inner wing spar without wing skin removal using Modified Principal Component Analysis. NDT E Int., 2013, 55: 21–27.Google Scholar
- He Y, Luo F, Pan M, et al. Pulsed eddy current technique for defect detection in aircraft riveted structures. NDT E Int., 2010, 43(2): 176–181.Google Scholar
- Abrantes R F, Rosado L S, Piedade M, et al. Pulsed eddy currents testing using a planar matrix probe. Measurement, 2016, 77: 351–361.Google Scholar
- Southwest Research Institute. Southwest Research Institute 2004 Annual Report, 2004.Google Scholar
- Yang G, Tamburrino A, Udpa L, et al. Pulsed eddy-current based giant magnetoresistive system for the Inspection of aircraft structures. IEEE Transactions on Magnetics, 2010, 46(3): 910–917.Google Scholar
- He Y, Pan M, Luo F, et al. Pulsed eddy current imaging and frequency spectrum analysis for hidden defect nondestructive testing and evaluation. NDT E Int., 2011, 44(4): 344–352.Google Scholar
- He Y, Luo F, Pan M, et al. Defect classification based on rectangular pulsed eddy current sensor in different directions. Sensors Actuators A Phys., 2010, 157(1): 26–31.Google Scholar
- Arjun V, Sasi B, Rao B P C, et al. Optimisation of pulsed eddy current probe for detection of sub-surface defects in stainless steel plates. Sensors Actuators A Phys., 2015, 226: 69–75.Google Scholar
- Zhou D, Wang J, He Y, et al. Influence of metallic shields on pulsed eddy current sensor for ferromagnetic materials defect detection. Sensors Actuators A Phys., 2016, 248: 162–172.Google Scholar
- Fan M, Cao B, Sunny A I, et al. Pulsed eddy current thickness measurement using phase features immune to liftoff effect. NDT E Int., 2017, 86: 123–131.Google Scholar
- Tumanski S. Induction coil sensors—a review. Meas. Sci. Technol., 2007, 18(3): R31–R46.Google Scholar
- Ripka P, Janosek M. Advances in magnetic field sensors. IEEE Sensors Journal, 2010, 10(6): 1108–1116.Google Scholar
- Herrera-May A L, Aguilera-Cortés L A, García-Ramírez P J, et al. Resonant magnetic field sensors based on MEMS technology. Sensors, 2009, 9(10): 7785.Google Scholar
- Li Y, Tian G Y, Simm A. Fast analytical modelling for pulsed eddy current evaluation. NDT E Int., 2008, 41(6): 477–483.Google Scholar
- Kim J, Yang G, Udpa L, et al. Classification of pulsed eddy current GMR data on aircraft structures,” NDT E Int., 2010, 43(2): 141–144.Google Scholar
- Cheng W. Pulsed eddy current testing of carbon steel pipes’ wall-thinning through insulation and cladding. J. Nondestruct. Eval., 2012, 31(3): 215–224.Google Scholar
- Albrecht J, Carls S, Robert S. Magnetoresistive Sensors for Nondestructive Evaluation. 10th SPIE International Symposium, Nondestructive Evaluation for Health Monitoring and Diagnostics, Conference 5770, 2005.Google Scholar
- Panaitov G, Krause H-J, Zhang Y. Pulsed eddy current transient technique with HTS SQUID magnetometer for non-destructive evaluation. Phys. C Supercond., 2002, 372–376: 278–281.Google Scholar
- Li Y, Yan B, Li D, et al. Gradient-field pulsed eddy current probes for imaging of hidden corrosion in conductive structures. Sensors Actuators A Phys., 2016, 238: 251–265.Google Scholar
- Joubert P Y, Le Diraison Y, Xi Z, et al. Pulsed eddy current imaging device for non destructive evaluation applications. Sensors, 2013 IEEE, 2013: 1–4.Google Scholar
- Joubert P Y, Le Diraison Y. Pulsed eddy current imager for the enhanced non destructive evaluation of aeronautical riveted assemblies. IEEE SENSORS 2014 Proceedings, 2014: 1188–1191.Google Scholar
- Majidnia S, Nilavalan R, Rudlin J. Investigation of an encircling Pulsed Eddy Current probe for corrosion detection. IEEE Sensors 2014 Proceedings, 2014: 835–838.Google Scholar
- Dai X W, Ludwig R, Palanisamy R. Numerical simulation of pulsed eddy-current nondestructive testing phenomena. IEEE Transactions on Magnetics, 1990: 26(6): 3089–3096.Google Scholar
- Ludwig R, Dai X W. Numerical and analytical modeling of pulsed eddy currents in a conducting half-space. IEEE Transactions on Magnetics, 1990: 26(1): 299–307.Google Scholar
- Allen B L, Lord W. Finite element modeling of pulsed eddy current phenomena. Review of Progress in Quantitative Nondestructive Evaluation, 1984: 3(A): 561–568.Google Scholar
- Allen B, Ida N, Lord W. Finite element modeling of pulse Eddy current NDT phenomena. IEEE Transactions on Magnetics, 1985, 21(6): 2250–2253.Google Scholar
- Desjardins D P R, Krause T W, Gauthier N. Analytical modeling of the transient response of a coil encircling a ferromagnetic conducting rod in pulsed eddy current testing. NDT E Int., 2013, 60: 127–131.Google Scholar
- Fan M, Huang P, Ye B, et al. Analytical modeling for transient probe response in pulsed eddy current testing. NDT E Int., 2009, 42(5): 376–383.Google Scholar
- Chen X, Lei Y. Time-domain analytical solutions to pulsed eddy current field excited by a probe coil outside a conducting ferromagnetic pipe. NDT E Int., 2014, 68: 22–27.Google Scholar
- Fan M, Cao B, Wang Y. Computation of coil-induced voltage due to a defect-free plate using Stehfest’s method for pulsed eddy current evaluation. Insight Non-Destructive Test. Cond. Monit., 2010, 52(6): 302–304.Google Scholar
- Chen X, Lei Y. Electrical conductivity measurement of ferromagnetic metallic materials using pulsed eddy current method. NDT E Int., 2015, 75: 33–38.Google Scholar
- Theodoulidis T, Wang H, Tian G Y. Extension of a model for eddy current inspection of cracks to pulsed excitations. NDT E Int., 2012, 47: 144–149.Google Scholar
- Liu S X, Xin W, Ding K Q. Simulation of corrosion on detection for pulsed eddy current. Fuzzy Systems and Knowledge Discovery (FSKD), 2010 Seventh International Conference on, 2010, 4: 1839–1842.Google Scholar
- Pavo J. Numerical calculation method for pulsed eddy-current testing. IEEE Transactions on Magnetics, 2002, 38(2): 1169–1172.Google Scholar
- Alamin M, Tian G Y, Andrews A, et al. Principal component analysis of pulsed eddy current response from corrosion in mild steel. IEEE Sensors Journal, 2012, 12(8): 2548–2553.Google Scholar
- Xu Z, Wu X, Li J, et al. Assessment of wall thinning in insulated ferromagnetic pipes using the time-to-peak of differential pulsed eddy-current testing signals. NDT E Int., 2012, 51: 24–29.Google Scholar
- Tian G Y, Sophian A. Defect classification using a new feature for pulsed eddy current sensors. NDT & E International, 2005, 38(1): 77–82.Google Scholar
- Chen X, Hou D, Zhao L, et al. Study on defect classification in multi-layer structures based on Fisher linear discriminate analysis by using pulsed eddy current technique. NDT E Int., 2014, 67: 46–54.Google Scholar
- BinFeng Y, FeiLu L, Dan H. Research on edge identification of a defect using pulsed eddy current based on principal component analysis. NDT E Int., 2007, 40(4): 294–299.Google Scholar
- Yang G, Tian G Y, Que P W, et al. Independent component analysis–based feature extraction technique for defect classification applied for pulsed eddy current NDE. Res. Nondestruct. Eval., 2009, 20(4): 230–245.Google Scholar
- Sophian A, Tian G Y, Taylor D, et al. A feature extraction technique based on principal component analysis for pulsed Eddy current NDT. NDT & E International, 2003, 36(1): 37–41.Google Scholar
- Horan P F, Underhill P R, Krause T W. Real time pulsed eddy current detection of cracks in F/A-18 inner wing spar using discriminant separation of modified principal components analysis scores. IEEE Sensors Journal, 2014, 14(1): 171–177.Google Scholar
- Qiu X, Zhang P, Wei J, et al. Defect classification by pulsed eddy current technique in con-casting slabs based on spectrum analysis and wavelet decomposition. Sensors Actuators A Phys., 2013, 203: 272–281.Google Scholar
- Pan M, He Y, Tian G, et al. Defect characterisation using pulsed eddy current thermography under transmission mode and NDT applications. NDT E Int., 2012, 52: 28–36.Google Scholar
- Stott C A, Underhill P R, Babbar V K, et al. Pulsed eddy current detection of cracks in multilayer aluminum lap loints. IEEE Sensors Journal, 2015, 15(2): 956–962.Google Scholar
- Buck J A, Underhill P R, Mokros S G, et al. Pulsed eddy current inspection of support structures in steam generators. IEEE Sensors Journal, 2015, 15(8): 4305–4312.Google Scholar
- Hosseini S, Lakis A A. Application of time–frequency analysis for automatic hidden corrosion detection in a multilayer aluminum structure using pulsed eddy current. NDT E Int., 2012, 47: 70–79.Google Scholar
- Qiu X B, Liu L L, Li C L, et al. Defect classification by pulsed eddy-current technique based on power spectral density analysis combined with wavelet transform. IEEE Trans. Magn., 2014, 50(9): 1–8.Google Scholar
- Kiwa T, Kawata T, Yamada H, et al. Fourier-transformed eddy current technique to visualize cross-sections of conductive materials. NDT E Int., 2007, 40(5): 363–367.Google Scholar
- Tian G Y, Sophian A, Taylor D, et al. Wavelet-based PCA defect classification and quantification for pulsed eddy current NDT. IEE Proceedings - Science, Measurement and Technology, 2005, 152(4): 141–148.Google Scholar
- Zhang Q, Chen T, Yang G, et al. Time and frequency domain feature fusion for defect classification based on pulsed eddy current NDT. Res. Nondestruct. Eval., 2012, 23(3): 171–182.Google Scholar
- Giguère S, Lepine B A, Dubois J M S. Pulsed eddy current technology: characterizing material loss with gap and lift-off variations. Res. Nondestruct. Eval., 2001, 13(3): 119–129.Google Scholar
- Giguère S, Dubois S J M. Pulsed eddy current: Finding corrosion independently of transducer lift-off. AIP Conf. Proc., 2000, 509(1): 449–456.Google Scholar
- Angani C S, Ramos H G, Ribeiro A L, et al. Lift-off point of intersection feature in transient eddy-current oscillations method to detect thickness variation in stainless steel. IEEE Transactions on Magnetics, 2016, 52(6): 1–8.Google Scholar
- Liu Z, Ramuhalli P, Safizadeh S, et al. Combining multiple nondestructive inspection images with a generalized additive model. Meas. Sci. Technol., 2008, 19(8): 817–822.Google Scholar
- Lefebvre J H V, Dubois J M S. Lift-off point of intercept (LOI) behavior. AIP Conference Proceedings, 2005, 760: 523–530.Google Scholar
- Tian G Y, Li Y, Mandache C. Study of lift-off invariance for pulsed eddy-current signals. IEEE Trans. Magn., 2009, 45(1): 184–191.Google Scholar
- Li Y B, Chen Z B, Qi Y. Generalized analytical expressions of liftoff intersection in PEC and a liftoff-intersection-based fast inverse model. IEEE Trans. Magn., 2011, 47(10): 2931–2934.Google Scholar
- Lefebvre J H V, Mandache C. Pulsed eddy current thickness measurement of conductive layers over ferromagnetic substrates. Int. J. Appl. Electromagn. Mech., 2008, 27(1–2): 1–8.Google Scholar
- Mandache C, Lefebvre J H V. Transient and harmonic eddy currents: Lift-off point of intersection. NDT E Int., 2006, 39(1): 57–60.Google Scholar
- Kral J, Smid R, Ramos H M G, et al. The lift-off effect in Eddy currents on thickness modeling and measurement. IEEE Trans. Instrum. Meas., 2013, 62(7): 2043–2049.Google Scholar
- Tian G Y, Sophian A. Reduction of lift-off effects for pulsed eddy current NDT. NDT E Int., 2005, 38(4): 319–324.Google Scholar
- Yu Y, Yan Y, Wang F, et al. An approach to reduce lift-off noise in pulsed eddy current nondestructive technology. NDT E Int., 2014, 63: 1–6.Google Scholar
- Huang C, Wu X. Probe lift-off compensation method for pulsed eddy current thickness measurement. Antennas and Propagation (APCAP), 2014 3rd Asia-Pacific Conference on., 2014: 937–939.Google Scholar
- Tian G Y, He Y, Adewale I, et al. Research on spectral response of pulsed eddy current and NDE applications. Sensors Actuators A Phys., 2013, 189: 313–320.Google Scholar
- Yang H-C, Tai C-C. Pulsed eddy-current measurement of a conducting coating on a magnetic metal plate. Meas. Sci. Technol., 2002, 13(8): 1259.Google Scholar
- Shin Y-K, Choi D-M, Kim Y-J, et al. Signal characteristics of differential-pulsed eddy current sensors in the evaluation of plate thickness. NDT E Int., 2009, 42(3): 215–221.Google Scholar
- Robers M A, Scottini R. Pulsed eddy currents in corrosion detection. NDT.net, 2002: 7(10).Google Scholar
- Eddyfi. Lyft Specifications Sheet. [Online]. Available: http://www.eddyfi.com/wp-content/uploads/2016/09/specifications-sheet-lyft.pdf. [Accessed: 02-Oct-2016].
- Xie S, Chen Z, Takagi T, et al. Quantitative non-destructive evaluation of wall thinning defect in double-layer pipe of nuclear power plants using pulsed ECT method. NDT E Int., 2015, 75: 87–95.Google Scholar
- Park D G, Angani C S, Kim G D, et al. Evaluation of pulsed eddy current response and detection of the thickness variation in the stainless steel. IEEE Transactions on Magnetics, 2009, 45(10): 3893–3896.Google Scholar
- Park D-G, Angani C S, Kishore M B, et al. The effects of lift-off from wall thinning signal in pulsed eddy current testing. J. Magn., 2012, 17(4): 298–301.Google Scholar
- Chen T, Tian G Y, Sophian A, et al. Feature extraction and selection for defect classification of pulsed eddy current NDT. NDT E Int., 2008, 41(6): 467–476.Google Scholar
- Lai S, Chen D Y, Chen H, et al. Pulsed eddy current testing of inner wall flaws in pipe under insulation. Procedia Eng., 130: 1658–1664.Google Scholar
- Tian G, He Y, Alamin M, et al. Corrosion characterisation using pulsed eddy current sensor systems. Sensing Technology (ICST), 2011 Fifth International Conference on., 2011: 498–503.Google Scholar
- Sophian A, Tian G Y, Taylor D, et al. Design of a pulsed eddy current sensor for detection of defects in aircraft lap-joints. Sensors Actuators, A Phys., 2002: 101(1–2): 92–98.Google Scholar
- Wu J, Zhou D, Wang J, et al. Surface crack detection for carbon fiber reinforced plastic (CFRP) materials using pulsed eddy current testing. Nondestructive Evaluation/Testing (FENDT), 2014 IEEE Far East Forum on., 2014: 181–185.Google Scholar
- He Y, Tian G, Pan M, et al. Non-destructive testing of low-energy impact in CFRP laminates and interior defects in honeycomb sandwich using scanning pulsed eddy current. Compos. Part B Eng., 59: 196–203.Google Scholar
- Morozov M, Tian G Yun, Withers P J. The pulsed eddy current response to applied loading of various aluminium alloys. NDT E Int., 2010, 43(6): 493–500.Google Scholar
- Rosado L S, Santos T G, Ramos P M, et al. A differential planar eddy currents probe: Fundamentals, modeling and experimental evaluation. NDT E Int., 2012: 51: 85–93.Google Scholar
- Zhou D, Wang J, Wu J, et al. Investigation of rectangular differential probes for pulsed eddy current non-destructive testing. Insight - Non-Destructive Test. Cond. Monit., 2016, 58(2): 87–100.Google Scholar
- Sergeeva-Chollet N, Decitre J, Fermon C, et al. Intrinsic noise study of Eddy current probes based on magnetoresistive sensors. 11th European Conference on Non-Destructive Testing (ECNDT 2014), 2014.Google Scholar
- Adewale I D, Tian G Y. Decoupling the influence of permeability and conductivity in pulsed eddy-current measurements. IEEE Transactions on Magnetics, 2013, 49(3): 1119–1127.Google Scholar
- Fan M, Cao B, Yang P, et al. Elimination of liftoff effect using a model-based method for eddy current characterization of a plate. NDT E Int., 2015, 74: 66–71.Google Scholar